Effect of the Size Distribution of Nanoscale Dispersed Particles
on the Zener Drag Pressure
A.R. EIVANI, S. VALIPOUR, H. AHMED, J. ZHOU, and J. DUSZCZYK
In this article, a new relationship for the calculation of the Zener drag pressure is described in which the eﬀect of the size distribution of nanoscale dispersed particles is taken into account, in addition to particle radius and volume fraction, which have been incorporated in the existing relationships. Microstructural observations indicated a clear correlation between the size distribution of dispersed particles and recrystallized grain sizes in the AA7020 aluminum alloy. However, the existing relationship to calculate the Zener drag pressure yielded a negligible diﬀerence of 0.016 pct between the two structures homogenized at diﬀerent conditions resulting in totally diﬀerent size distributions of nanoscale dispersed particles and, consequently, recrystallized grain sizes. The diﬀerence in the Zener drag pressure calculated by the application of the new relationship was 5.1 pct, being in line with the experimental observations of the recrystallized grain sizes. Mathematical investigations showed that the ratio of the Zener drag pressure from the new equation to that from the existing equation is maximized when the number densities of all the particles with diﬀerent sizes are equal. This ﬁnding indicates that in the two structures with identical parameters except the size distribution of nanoscale dispersed particles, the one that possesses a broader size distribution of particles, i.e., the number densities of particles with diﬀerent sizes being equal, gives rise to a larger Zener drag pressure than that having a narrow size distribution of nanoscale dispersed particles, i.e., most of the particles being in the same size range.
The Author(s) 2010. This article is published with open access at Springerlink.com
DISPERSED second-phase particles exert a retard-ing force or pressure, named Zener drag, on the low-and high-angle grain boundaries, which signiﬁcantly aﬀects the recovery, recrystallization, and grain growth of deformed structures.[1–10]It is commonly understood that the Zener drag pressure is a complex function of the interface, shape, size, interspacing, and volume fraction of dispersed particles.[1,2]
One of the primary objectives of the homogenization treatment applied to direct-chill cast aluminum alloys before hot deformation is to create small dispersoids that act as recrystallization inhibitors during deforma-tion and annealing or soludeforma-tion treatments.In 3XXX series aluminum alloys, e.g., Mn-containing dispersoids formed during homogenization, play an important role in controlling the recrystallization behavior of the alloys.[12,13] In 6XXX series aluminum alloys, the formation of diﬀerent kinds of dispersoids, i.e., Zr-,
Mn-, and Cr-containing ones, which play a role of recrystallization inhibition, has been investigated.[14–18] In the case of 7XXX series aluminum alloys, the formation of Zr- and Sc-containing dispersoids has been a subject of interest for many years.[19–21] For example, Robson et al.[19,20]investigated the eﬀect of Zr addition on the dispersoid formation and the fraction recrystallized after hot deformation. It was concluded that by using an optimum two-step homogenization treatment, a smaller fraction of recrystallization could be obtained. Robsonalso studied the eﬀect of Sc on the formation of dispersoids, as Sc was expected to eliminate the dispersoid-free zones, as observed in scandium-free 7050, thus greatly increasing the recrys-tallization resistance. Other investigations showed that, in addition to the size, shape, and volume fraction of dispersed particles, their size distribution is dependent on the homogenization treatment. For example, Fuller and Seidman[22,23]investigated the precipitation and the evolution of Al(Sc,Zr) particles in an Al-Sc-Zr alloy during heat treatment and found these particles with diﬀerent size distributions after diﬀerent treatments. The results obtained by Clouet et al.also clearly showed that quite diﬀerent size distributions of Al3Zr and Al3Sc particles ranging from a broad distribution to a local-ized one might result from diﬀerent treatments employed. Similar observations were made by Li and Arnbergas to the formation of Mn-rich dispersoids in the AA3003 aluminum alloy and by Novotny and Ardellconcerning the formation of Al3Sc particles in an Al-Sc alloy.
A.R. EIVANI, Researcher, is with the Materials Innovation Institute, 2628 CD Delft, The Netherlands, and the School of Metallurgical and Materials Engineering, Iran University of Science and Technology (IUST), Tehran, Iran. Contact e-mail: a.eivani@ m2i.nl S. VALIPOUR, Researcher, is with the School of Science, Razi University, Kermanshah, Iran. H. AHMED, Researcher, is with the Materials Innovation Institute. J. ZHOU and J. DUSZCZYK, Associate Professors, are with the Department of Materials Science and Engineering, Delft University of Technology, 2628 CD Delft, The Netherlands.
Manuscript submitted May 7, 2009. Article published online November 17, 2010
Considering a random spatial correlation between the boundaries and the dispersed particles, the Zener drag pressure (Pz) can be expressed in the simplest form by the following relationship:[1,2]
where Fv is the local volume fraction of dispersed particles, r the particle radius, and c the energy of the grain boundary that dispersed particles are pinning. It can be seen from Eq.  that the Zener drag due to the presence of dispersed particles at grain boundaries is maximized by maximizing the volume fraction (Fv) and minimizing the particle size (r).
There are also some interesting publications on the eﬀect of Zener drag pressure on the recrystallization behavior. For example, Nes et al.studied the interac-tions between particles and grain boundaries, including the eﬀects of the size, shape, and distribution of the particles with the same size, and found that such eﬀects may strongly aﬀect the recrystallization and grain growth. However, the authors did not consider the eﬀect of the size distribution of particles. Andersen and Grong[27,28] proposed an analytical model of grain growth in metals and alloys in the presence of growing and dissolving precipitates on normal and abnor-mal grain growth. Novikov simulated the grain growth in three-dimensional model polycrystals with randomly distributed particles at the grain boundaries. The particles were assumed to be of spherical shape and identical sizes, and their boundaries to be noncoherent. Simulations yielded the exact dependence of the normal-ized limiting grain size on the particle volume fraction, regardless of the initial grain size. It was concluded that in materials with randomly distributed particles, the dependence of the normalized limiting grain size on the volume fraction is tight up to a volume fraction of 0.12, which proved the validity of the Zener theory as well as their simulations. Maazi and Rouag presented a model for grain growth simulation, in the presence of a preferential particle distribution. The model predicted two grain size limits due to second-phase particles. If the particles had a size less than the maximal critical radius, the grains would shrink, and if these had a size greater than the minimal critical radius, the grains would grow, while between the two limiting radii, no grain growth took place. In most of the studies in this ﬁeld, the basic equation of Eq.  and its derivations[6–9]have been used to estimate the retarding pressure for recrystallization, and a reasonable agreement between the predictions and the experimental results has been reached. Further studies[8,11,12] on the Zener drag without introducing other eﬀective parameters such as the size distribution of dispersed particles have not led to any relationship that is signiﬁcantly diﬀerent from Eq. .
In other studies, however, the size distribution of dispersed particles has been recognized as an eﬀective parameter on the physical and mechanical behavior of materials. For example, the eﬀect of the size distribution of dispersed particles on the mechanical properties and the growth and dissolution of these particles in struc-tures were investigated.[31–36]Myhr et al.generated a
special control volume formulation of the classical precipitation model for coupled nucleation, growth, and coarsening to describe the evolution of the particle size distribution with time during thermal processing of Al-Mg-Si alloys, including both isothermal and noniso-thermal transformation behavior. The size distribution of particles was found to be eﬀective on the precipitation behavior. Myhr and Grong studied the nonisother-mal transformations in alloys containing a distribution of particles and found that the memory of a past process step, i.e., the previous particle sizes, is likely to have an eﬀect on the overall transformation behavior. In addi-tion, Tundal and Ryum[35,36] investigated the eﬀect of size distribution of dispersed particles on their dissolu-tion during homogenizadissolu-tion. It was demonstrated that the size distribution of particles is an eﬀective parameter on the model predictions and, therefore, should be considered in the model if an accurate prediction of the dissolution kinetics is to be achieved. However, there has been no publication on the eﬀect of size distribution of dispersed particles on the recrystallization behavior. In other words, no study has been conducted with the eﬀect of this parameter on the Zener drag pressure taken into account, although it is experimentally observed that this eﬀect is partly responsible for recrystallization and grain growth behavior.
In this article, two heating rates toward a homogeni-zation temperature were chosen in order to create two distinctively diﬀerent size distributions of dispersed particles with similar values of Pz based on Eq. . The samples were then hot deformed, followed by annealing to demonstrate a relationship between the size distribution of dispersed particles and the recrystallized grain size in the AA7020 aluminum alloy. The objective of this research was to derive a new relationship that included the eﬀect of the size distribution of dispersed particles in the calculation of the Zener drag pressure. The derived equation could then be used to suggest an optimum size distribution of dispersed particles, which would result in a maximum Zener drag pressure.
II. EXPERIMENTAL PROCEDURE
Cubic samples of 20 mm were cut from the center of a direct chill cast AA7020 ingot. The chemical composi-tion of the samples used in this study is shown in TableI. The as-cast samples were homogenized at 783 K (510C) for 8 hours prior to which two diﬀer-ent heating rates of 523 K and 323 K/h (250C and 50C/h) were applied and coded as S1 and S2. After the homogenization treatment, the samples were cooled in air.
The as-homogenized samples were examined using a JEOL* 6500 ﬁeld emission gun–scanning electron
microscope (FEG-SEM). The optimum operating voltage and current were found to be 10 kV and 1 nA, respectively. To estimate the number density of
nanoscale dispersed particles, images at a magniﬁcation of 50,000 were examined using image analysis, while for the determination of the sizes of the dispersed particles, a magniﬁcation of 75,000 was used in order to ensure accuracy.
Uniaxial hot compression tests were performed at 723 K (450C) at a strain rate of 10 s1, using a DSI GLEEBLE** 3800 thermomechanical simulator.
Compressive deformation proceeded to a strain of 0.6. The tests were performed at least twice for each condition to ensure the repeatability of the data. Cylindrical samples having a diameter of 10 mm and a length of 12 mm were used. They were heated to 723 K (450 C) at a heating rate of 10 K/s (10 C/s) and kept at the temperature for 110 seconds in order to attain a homogenous temperature in the test material and anvils, based on the previous studies using the same facility. The samples were subsequently water quenched to maintain the as-deformed structure so that no further microstructural changes would occur after deformation. The samples were annealed in a salt bath furnace at 773 K (500C) for 2 hours and then cut through thickness. The grain structure was studied by a polarized light optical microscope. The average grain size from ﬁve images was determined using the general line intercept procedure according to ASTM E 112-96.
III. RESULTS AND DISCUSSION
A. Effective Parameters on the Recrystallization Resistance and Grain Growth
The ability of FEG-SEM to determine the sizes of dispersoids of larger than 10 nm in AA7050 has been reported. In addition, it has been conﬁrmed by the present authors in the case of AA7020 that the particle radii measured using both FEG-SEM and transmission electron microscopy imaging methods are in quite reasonable agreement. However, the FEG-SEM is easier to use and gives the possibility of investigating a larger area of sample for statistical measurements and was thus used exclusively in this investigation.
Figures1(a) and 2(a) present typical FEG-SEM images of samples S1 and S2, respectively. The white spots clearly seen in the images are the dispersed particles, which have distinctly diﬀerent distributions as a result of the diﬀerent homogenization conditions. The size distributions of the particles are shown in Figures1(b) and 2(b). It can be seen that these two structures indeed contain dispersed particles of quite diﬀerent size distributions. It should be mentioned that the sizes of individual particles in each image were measured by taking pictures at higher magniﬁcations under the SEM. In sample S1, most of the particles fall in a narrow size range of 26 to 30 nm, while in sample S2, the number densities of the particles with diﬀerent sizes from 14 to 40 nm are almost equal. The main reason for these two diﬀerent particle size distributions is the diﬀerent heating rates applied during homogeni-zation from room temperature to the homogenihomogeni-zation temperature. At the faster heating rate, sample S1, the material was taken to the homogenization temperature within a short period of time, about 1 hour. In this case, most of the dispersoids formed at higher temperatures, near or at 783 K (510C). At these temperatures, the critical radius for a new nucleus to form is larger than at Table I. Chemical Composition of the Alloy Used
in this Study
Element Si Fe Cu Mn Mg Zn Ti Cr Zr Al
Wt pct 0.30 0.30 0.19 0.35 1.20 4.37 0.002 0.10 0.13 bal.
Fig. 1—(a) FEG-SEM image of the sample S1 after the homogenization treatment and (b) average size distribution of the nanoscale dispersed particles determined from 25 images. N = 5.3 lm2(N = 12.2 lm3) and raveg= 30 nm.
lower temperatures.[40–42] It is possible that some of the nuclei that formed during heating would dissolve in the structure, since at the homogenization temperature, they might not be stable at 783 K (510C). Such behavior has been observed in the case of the formation of precipitates during age hardening of aluminum alloys.[33–36] Therefore, only the particles that had suﬃciently large sizes could survive and continue to grow, which resulted in a narrow size distribution of particles. In addition, due to the very short time to reach the homogenization temperature, the fraction of the particles that formed during heating might not be signiﬁcant. Therefore, most of the particles formed near or at the homogenization temperature and, conse-quently, had almost the same sizes. However, at the lower heating rate, sample S2 was at low temperatures for a longer time during heating, about 10 hours compared to 1 hour for S1. Particles having diﬀerent sizes would form during heating and became stable before reaching the homogenization temperature. Con-sequently, sample S2 had almost equal number densities of particles with diﬀerent sizes.
The average particle radii and number densities are shown in Table II, which also presents the average normalized values of the Zener drag pressure (Pz/c), calculated using Eq. . It is clear that although these two microstructures contain dispersed particles with quite diﬀerent size distributions, Eq.  results in very
similar Pz/c values with a diﬀerence as small as 0.016 pct. (This value has been calculated as the percentage diﬀerence between the values of Pz/c in samples S1 and S2.)
To verify the viability of the existing relationship, Eq. , to calculate the Zener drag pressure, the recrystallization response of the samples after hot deformation and annealing was investigated and the results are shown in Figures3(a) and (b) for the samples S1 and S2, respectively. It is clear that the sample S2 heated at a slower rate to the homogenization temper-ature of 783 K (510C) has smaller recrystallized grains. S2 has an average grain size of 54 ± 5 lm, while S1 has an average grain size of 73 ± 7 lm.
It is well known that the interface, shape, size, interspacing, and volume fraction of dispersed parti-cles[1,2]aﬀect the Zener drag pressure and, therefore, the recrystallization resistance and grain growth of a deformed material. The Zener drag pressure exerted by dispersed particles shown in Eq.  represents the easiest way to judge the recrystallization resistance of the deformed material. However, the results of the present investigation clearly show that in spite of the similar values of the Zener drag pressure based on the existing relationship (Eq. ), the recrystallization response is quite diﬀerent. This indicates that in addition to the mentioned parameters, the size distribution of dispersed particles may also be eﬀective on the recrystallization resistance.
B. The Zener Drag Relationship Including the Effect of the Size Distribution of Dispersed Particles
The procedure to calculate the Zener drag pressure including the size distribution of particles was the same as that used in References and. Assuming that the boundary is planar,[1,2]the particle within a distance ri
Fig. 2—(a) FEG-SEM image of the sample S2 after the homogenization treatment and (b) average size distribution of the nanoscale dispersed particles determined from 25 images. N = 5.94 lm2(N = 14.48 lm3) and raveg= 28 nm.
Table II. Number Densities and Average Radii of Nanoscale Dispersed Particles, along with the Calculated
Pz/c Values Using Equation 
Sample Name N(lm3) raveg (nm) Pz/c (lm1) Difference in Pz/c (Pct) S1 12.20 30 0.06894 0.016 S2 14.48 28 0.06895
on either side of the boundary will intersect it. There-fore, NSi, the number of particles intersecting with a unit area of the boundary for the particles with a size of ri, is[1,2]
NSi¼ 2riNVi ½2
where Nviis the number of particles with a radius of ri per unit volume. The pinning pressure exerted on the unit area of the boundary by the particles with a size of ri(PZi) is given by[1,2]
PZi¼ NSiFSi ½3
in which, the maximum restraining force on the boundary, FSi, can be expressed as[1,2]
FSi¼ pric ½4
where c is the speciﬁc energy of the boundaries that the particles pin. Equation  may be rewritten as[1,2]
PZi ¼ NSipric ½5 Inserting Eq.  into Eq.  leads to
PZi¼ 2NVipr2ic ½6 Therefore, the pressure exerted on a boundary by a group of particles with diﬀerent sizes is
By inserting the relationship between the number den-sity of particles, their radii, and the volume fraction presented in Eq. [1,2]into Eq. , Eq.  is derived.
NVi¼ 3FVi 4pr3 i ½8 PZ¼ 3 2c Xn i¼1 FVi ri ½9
TableIII shows the calculated normalized values of the Zener drag pressure (Pz/c) for samples S1 and S2,
based on Eq. . It is clear that the newly derived equation predicts a larger value of Pz/c for sample S2, being 5.1 pct larger than that of sample S1, which is in line with the experimental observations in this research. As mentioned earlier, the percentage is expressed by the percentage diﬀerence between the values of Pz/c in samples S1 and S2.
C. Differences between the Existing and the Newly Derived Equations
Based on Eq. , it is clear that the newly derived equation is inherently close to the existing one, Eq. . However, Eq.  gives the possibility to diﬀerentiate between diﬀerent size distributions of particles to obtain the highest recrystallization inhibition. The term a is deﬁned as the ratio of the Zener drag pressure including the eﬀect of the size distribution of dispersed particles to the Zener drag pressure without this eﬀect. For the a parameter, the Zener drag pressure was calculated using the average radius of the dispersed particles, following the same procedure, which resulted in
PZavg¼ 2pcNVavgr2avg ½10 where NVavg¼ Xn i¼1 NVi ½11 and ravg¼ Pn i¼1 NViri Pn i¼1 NVi ½12
Fig. 3—Grain structure after annealing at 848 K (575C) for 10 min, following hot compression tests of the samples (a) S1 and (b) S2.
Table III. Calculated Pz/c Values for Samples S1 and S2
Using Equation 
Sample Name Pz/c (lm1) Difference in Pz/c (Pct)
S1 0.0726 5.1
Therefore, substituting the terms in Eq.  with Eqs.  and  yields a Pzvalue equal to
PZavg¼ 2pc Pn i¼1 NViri 2 Pn i¼1 NVi ½13 The a parameter is a¼ PZ PZavg ¼ Pn i¼1 NVir2i Pn i¼1 NVi Pn i¼1 NViri 2 ½14
With mathematical simpliﬁcation, Eq.  may be rewritten as a¼ Pn i¼1 NViri 2 þP n1 i¼1 NVi P n j¼iþ1 NVjri rj 2 ! Pn i¼1 NViri 2 ½15
The detailed expressions of the individual terms in Eq.  are presented in Appendix A. Assuming the dispersed particles with diﬀerent sizes are at a constant size diﬀerence equal to d, i.e., (ri+1– ri) = d, a may be expressed as a¼ Pn i¼1 NViri 2 þd2n1P i¼1 NVi P n j¼iþ1 NVj ! Pn i¼1 NViri 2 ½16
It is clear that the ﬁrst term of the numerator in Eq.  is equal to the denominator. Therefore, the determining term for the maximization of the a parame-ter is the second parame-term of the numerator deﬁned as NUM.
NUM¼ d2X n1 i¼1 NVi Xn j¼iþ1 NVj ! ½17
Since all the terms in Eq.  are positive, a is always larger than 1. This ﬁnding indicates that the newly derived equation for the Zener drag pressure always has a larger value than the one using the average parti-cle size values. This may be considered an advantage over the Pzcalculated from the average values, since it is always less than the values predicted by the equation according to the size distribution of particles. In other words, it is a trustable equation to rely on for inhibit-ing recrystallization. As presented in Appendix B, NUM will be maximized when the number densities of the particles of diﬀerent sizes are equal, which may be written as
N1¼ N2¼ . . . ¼ Nmax¼ . . . ¼ Nn1¼ Nn ½18 Equation  indicates that for a given total number density of evenly dispersed particles, Pz is maximized when the particles with diﬀerent sizes have equal
number densities, as indicated by a broad distribution of particle sizes in the size distribution plot. This is in agreement with the ﬁnding in this research that the recrystallization resistance of sample S2 with a broader size distribution of particles, as shown in Figure 2(b), is larger. The corresponding values of the a parameter for samples S1 and S2 were calculated to be 1.05 and 1.11, respectively.
In this study, two diﬀerent homogenization treat-ments were applied, resulting in distinctively diﬀerent size distributions of dispersed particles. However, the Zener drag pressure values based on the existing equation showed only a very small diﬀerence of 0.016 pct, although the recrystallized grain sizes after hot deformation and subsequent annealing were quite diﬀerent. A new relationship for the Zener drag pressure was derived, which accounted for the eﬀect of the size distribution of dispersed particles. The predictions of the newly derived equation were compared to the recrystal-lized grain sizes after hot compression and subsequent annealing. The following conclusions have been drawn.
1. In addition to the known parameters, i.e., the inter-face, shape, size, interspacing, and volume fraction of dispersed particles, the size distribution of parti-cles is also an effective parameter on the recrystalli-zation inhibition of the alloy.
2. The newly developed equation is able to diﬀerenti-ate between the samples with similar Pzvalues from
the average particle radii, but with different size dis-tributions of dispersed particles.
3. The ratio of the Zener drag pressure from the new equation to that from the existing equation is maxi-mized when the number densities of all the particles with diﬀerent sizes are equal. This indicates that in the two structures with identical parameters except the size distribution of dispersed particles, the one that possesses a broader size distribution of parti-cles, i.e., the number densities of particles with dif-ferent sizes being equal, gives rise to a larger Zener drag pressure than that having a narrow size distri-bution of dispersed particles, i.e., most of the parti-cles being in the same small size range.
This research was carried out under Project No. MC 4.04203 in the framework of the Research Program of the Materials innovation institute M2i (www.m2i.nl).
This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distri-bution, and reproduction in any medium, provided the original author(s) and source are credited.
For the a parameter, Eq.  may be written as
a¼ N1r21þ N2r22þ N3r23þ . . . þ Nnr2n N1þ N2þ N3þ . . . þ Nn ð Þg= X n i¼1 NViri !2 ½A1
Multiplication in the numerator of Eq. [A1] leads to
a¼ N21r21þ N22r22þ N23r23þ . . . þ N2nr 2 n þ N1N2r21þ N1N3r21þ . . . þ N1Nnr21 þ . . . þ N nN1r2nþ NnN1r2nþ . . . þ NnNn1r2n= Xn i¼1 NViri !2 ½A2
Equation [A2] can be ordered as
a¼ N21r21 þN2 2r22 þN23r23 þ . . . þN2nr2n 0 B B B B B B B @ 1 C C C C C C C A þ N1N2 r21þ r 2 2 þN1N3 r21þ r23 þ . . . þN1Nn r21þ r2n 0 B B B B @ 1 C C C C A 8 > > > > > > > < > > > > > > > : þ N2N3 r22þ r 2 3 þN2N4 r22þ r24 þ . . . þN2Nn r22þ r2n 0 B B B B @ 1 C C C C Aþ N3N4 r23þ r 2 4 þN3N5 r23þ r25 þ . . . þN3Nn r23þ r2n 0 B B B B @ 1 C C C C A þ . . . þ Nn1Nn r2n1þ r2n 9 > > > > > > > = > > > > > > > ; , Xn i¼1 NViri !2 ½A3
which can be rearranged as
a¼ N21r21þ N2 2r22þ N23r23þ . . . þ N2nr2n þ 2Nð 1N2r1r2þ 2N1N3r1r3þ . . . þ 2N1Nnr1rnÞ þ 2Nð 2N3r2r3þ 2N2N4r2r4þ . . . þ 2N2Nnr2rnÞ þ 2Nð 3N4r3r4þ 2N3N5r3r5þ . . . þ 2N3Nnr3rnÞ þ . . . þ 2Nn1Nnrn1rng þ N1N2ðr1 r2Þ2þN1N3ðr1 r3Þ2þ . . . n þN1Nnðr1 rnÞ2 þ N2N3ðr2 r3Þ2þN2N4ðr2 r4Þ2þ . . . þN2Nnðr2 rnÞ2 þ N3N4ðr3 r4Þ2þN3N5ðr3 r5Þ2þ . . . : þN3Nnðr3 rnÞ2Þ þ . . . þ Nn1Nnðrn1 rnÞ2 o. Xn i¼1 NViri !2 ½A4 or a¼ X n i¼1 NViri !2 þ N1N2ðr1 r2Þ2þN1N3ðr1 r3Þ2 8 < : þ . . . þ N1Nnðr1 rnÞ2 þ N2N3ðr2 r3Þ2þN2N4ðr2 r4Þ2þ . . . þN2Nnðr2 rnÞ2 þ N3N4ðr3 r4Þ2þN3N5ðr3 r5Þ2þ . . . þN3Nnðr3 rnÞ2 þ . . . þ Nn1Nnðrn1 rnÞ2 9 = ; , Xn i¼1 NViri !2 ½A5
Eq. [A5] can be mathematically simpliﬁed as
a¼ Pn i¼1 NViri 2 þP n1 i¼1 NVi P n j¼iþ1 NVjri rj 2 ! Pn i¼1 NViri 2 ½A6
Assuming the dispersed particles with diﬀerent sizes are evenly sized with a diﬀerence equal to d, i.e., (ri– ri+1) = d = cte. a¼ Pn i¼1 NViri 2 þd2n1P i¼1 NVi P n j¼iþ1 NVj ! Pn i¼1 NViri 2 ½A7 APPENDIX B
Assuming the total number density of dispersed particles is Ntot, which can be written as
Ntot¼ N1þ N2þ . . . þ Nmaxþ . . . þ Nn1þ Nn ½B1 where Nmax is the largest number density of dispersed particles with a speciﬁc size, Eq. [B2] expressing the ratio of other number densities to the maximum number densities can be written as
Nmax¼ 1 m1 N1 ¼ 1 m2 N2¼ . . . ¼ 1 mn1 Nn1¼ 1 mn Nn ½B2
The numbers m1, m2,…, mn–1and mnshould be less than 1, since Nmaxis larger than all the other values of N, i.e., N1to Nn. Since the number density cannot have a negative value, m1, m2,…, mn–1, and mnshould be larger than zero. Equation  can be extended as
NUM¼ d2½ðN1N2þ N1N3þ . . . þ N1NnÞ
þ Nð 2N3þ N2N4þ . . . þ N2NnÞ
þ Nð 3N4þ N3N5þ . . . þ N3NnÞ
þ . . . þ Nn1Nn ½B3 Insertion of Nmaxinto Eq. [B3] yields
maxððm1m2þ m1m3þ . . . þ m1mnÞ
þ mð 2m3þ m2m3þ . . . þ m2mnÞ
þ mð 3m4þ m3m5þ . . . þ m3mnÞ
þ . . . þ mn1mnÞ ½B4
NUM in Eq. [B3] will be maximized if m1= m2=… = mn= 1, since m1 to mn are between 0 and 1. By giving 1 for all m1 to mn in Eq. [B2], it becomes
Nmax¼ N1¼ N2 ¼ . . . ¼ Nn1¼ Nn ½B5 This indicates that for a given total number density of evenly sized dispersed particles with a constant diﬀer-ence in size, Pz will be maximized when the particles with diﬀerent sizes have equal number densities.
1. F.J. Humphreys and M. Hatherly: Recrystallization and Related Annealing Phenomena, Elsevier Science, Inc., Oxford, United Kingdom, 1995, pp. 109–14.
2. E. Nes, N. Ryum, and O. Hunderi: Acta Metall., 1985, vol. 33, pp. 11–22.
3. M. Jones and F.J. Humphreys: Acta Mater., 2003, vol. 51, pp. 2149–59.
4. M. Ferry: Acta Mater., 2005, vol. 53, pp. 773–873. 5. C.S. Smith: Trans. TMS-AIME, 1948, vol. 175, pp. 15–51. 6. M.F. Ashby, J. Harper, and J. Lewis: Trans. TMS-AIME, 1969,
vol. 245, pp. 413–20.
7. R.D. Doherty, D.A. Hughes, F.J. Humphreys, J.J. Jonas, D. Juul Jensen, D.E. Kassner, W.E. King, T.R. McNelley, H.J. McQueen, and A.D. Rollett: Mater. Sci. Eng., 1997, vol. 238, pp. 219–74. 8. M. Hillert: Acta Metall., 1965, vol. 13, pp. 227–38.
9. F.J. Humphreys and M.G. Ardakani: Acta Mater., 1996, vol. 44, pp. 2717–27.
10. F.J. Humphreys: Acta Mater., 1997, vol. 45, pp. 5031–39. 11. T. Sheppard: Extrusion of Aluminum Alloys, Kluwer Academic
Publishers, Dordrecht, The Netherlands, 1999, pp. 227–52. 12. M. Peters, J. Eschweiler, and K. Welpmann: Scripta Metall., 1986,
vol. 20, pp. 259–64.
13. O. Daaland and E. Nes: Acta Mater., 1996, vol. 44, pp. 1389–1411.
14. L. Lodgaard and N. Ryum: Mater. Sci. Eng. A, 2000, vol. 283, pp. 144–52.
15. M. Cabibbo, E. Evangelista, C. Scalabroni, and E. Bonetti: Mater. Sci. Forum, 2006, vols. 503–504, pp. 841–46.
16. L. Lodgaard and N. Ryum: Mater. Sci. Technol., 2000, vol. 16, pp. 599–604.
17. D.H. Lee, J.H. Park, and S.W. Nam: Mater. Sci. Technol., 1999, vol. 15, pp. 450–55.
18. R.A. Jeniski, B. Thanaboonsombut, and T.H. Sanders: Metall. Mater. Trans. A, 1996, vol. 27A, pp. 19–27.
19. J.D. Robson and P.B. Prangnell: Acta Mater., 2001, vol. 49, pp. 599–613.
20. J.D. Robson: Mater. Sci. Eng. A, 2002, vol. 338, pp. 219–29. 21. J.D. Robson: Acta Mater., 2004, vol. 52, pp. 1409–21.
22. C.B. Fuller and D.N. Seidman: Acta Mater., 2005, vol. 53, pp. 5401–13.
23. C.B. Fuller and D.N. Seidman: Acta Mater., 2005, vol. 53, pp. 5415–28.
24. E. Clouet, A. Barbu, L. Lae, and G. Martin: Acta Mater., 2005, vol. 53, pp. 2313–25.
25. Y.J. Li and L. Arnberg: Acta Mater., 2003, vol. 51, pp. 3415–28. 26. G.M. Novotny and A.J. Ardell: Mater. Sci. Eng. A, 2001, vol. 318,
27. I. Andersen and Ø. Grong: Acta Metall. Mater., 1995, vol. 43, pp. 2673–88.
28. I. Andersen and Ø. Grong: Acta Metall. Mater., 1995, vol. 43, pp. 2689–2700.
29. V.Y. Novikov: Scripta Mater., 2000, vol. 42, pp. 439–43. 30. N. Maazi and N.J. Rouag: Cryst. Growth, 2002, vol. 243,
31. E. Nes: Proc. Symp. on Microstructural Control during Processing of Aluminum Alloys, New York, NY, 1985, pp. 95–102.
32. R.D. Doherty, D.J. Srolovitz, A.R. Rollet, and M.P. Anderson: Scr. Metall., 1987, vol. 21, pp. 675–79.
33. O.R. Myhr, Ø. Grong, and S.J. Andersen: Acta Mater., 2001, vol. 49, pp. 65–75.
34. O.R. Myhr and Ø. Grong: Acta Mater., 2000, vol. 48, pp. 1605–15. 35. U.H. Tundal and N. Ryum: Metall. Trans. A, 1992, vol. 23A,
36. U.H. Tundal and N. Ryum: Metall. Trans. A, 1992, vol. 23A, pp. 445–49.
37. F.A. Sloof, J. Zhou, and J. Duszczyk: 7th Int. Conf. Magnesium Alloys and Their Applications, Wiley-VCH, Weinheim, Germany, 2006, pp. 324–29.
38. ‘‘ASTM E 112-96 Standard Test Methods for Determining Average Grain Size,’’ Annual Book of ASTM Standards, ASTM International, West Conshohocken, PA, 2004, vol. 03.01, pp. 1–26.
39. A.R. Eivani, H. Ahmed, J. Zhou, J. Duszczyk, and C. Kwakernaak: Mater. Sci. Technol., 2010, in press, DOI
40. J.W. Martin: Precipitation Hardening, 2nd ed., Butterworth-Heinemann, Oxford, United Kingdom, 1998, pp. 79–111. 41. D.A. Porter and K.E. Easterling: Phase Transformation in Metals
and Alloys, VNR International, London, 1981, pp. 263–381. 42. R.W. Cahn and P. Haasen: Physical Metallurgy, 4th ed., Elsevier
Science BV, North Holland, the Netherlands, 1996, pp. 1363– 1400.